Embed Size (px)
Transcript of Problematica Hidrogeno
This document was prepared in conjunction with work accomplished under Contract No. DE-AC09-96SR18500 with the U.S. Department of Energy. This work was prepared under an agreement with and funded by the U.S. Government. Neither the U. S. Government or its employees, nor any of its contractors, subcontractors or their employees, makes any express or implied: 1. warranty or assumes any legal liability for the accuracy, completeness, or for the use or results of such use of any information, product, or process disclosed; or 2. representation that such use or results of such use would not infringe privately owned rights; or 3. endorsement or recommendation of any specifically identified commercial product, process, or service. Any views and opinions of authors expressed in this work do not necessarily state or reflect those of the United States Government, or its contractors, or subcontractors.
Hydrogen Embrittlement of Metals: A Primer for the Failure Analyst
M. R. Louthan, Jr.
Materials Science and Technology Savannah River National Laboratory
Aiken, South Carolina 29808 Abstract Hydrogen reduces the service life of many metallic components. Such reductions may be manifested as blisters, as a decrease in fatigue resistance, as enhanced creep, as the precipitation of a hydride phase and, most commonly, as unexpected, macroscopically brittle failure. This unexpected, brittle fracture is commonly termed hydrogen embrittlement. Frequently, hydrogen embrittlement occurs after the component has been is service for a period of time and much of the resulting fracture surface is distinctly intergranular. Many failures, particularly of high strength steels, are attributed to hydrogen embrittlement simply because the failure analyst sees intergranular facture in a component that served adequately for a significant period of time. Unfortunately, simply determining that a failure is due to hydrogen embrittlement or some other form of hydrogen induced damage is of no particular help to the customer unless that determination is coupled with recommendations that provide pathways to avoid such damage in future applications. This paper presents qualitative and phenomenological descriptions of the hydrogen damage processes and outlines several metallurgical recommendations that may help reduce the susceptibility of a particular component or system to the various forms of hydrogen damage. Introduction The ASM Materials Handbook lists five specific types of hydrogen induced damage to metals and alloys. These types are:
1) hydrogen embrittlement, 2) hydrogen-induced blistering 3) cracking from precipitation of internal hydrogen, 4) hydrogen attack, and 5) cracking from hydride formation.
Except for hydrogen embrittlement, a phase transformation is coupled to each of the listed hydrogen damage process. The forms of hydrogen damage that involve phase transformations are relatively easy to understand in a qualitative fashion and may be minimized by simply paying attention to the damage causing process. Understanding the damage process involved in hydrogen embrittlement is much more elusive and avoiding the damage processes has proven difficult. However, there are several general metallurgical trends that can be helpful in the prevention of hydrogen embrittlement failures.
This paper provides a qualitative description of the four hydrogen damage processes that involve a phase transformation and a phenomenological description of hydrogen embrittlement. Additionally, a brief description of hydrogen absorption by, and migration (diffusion) in, metals is included as an aid to understanding some of the hydrogen induced damage processes. Background Hydrogen dissolves in metals as an atom or screened proton rather than as a hydrogen molecule. Therefore, the absorption of hydrogen requires the presence of atomic (nascent) hydrogen on the metal surface. The formation of nascent hydrogen on a metal surface exposed to a gaseous hydrogen environment requires the disassociation of hydrogen molecules as illustrated schematically by Figure 1. The amount of hydrogen absorbed will depend on the efficiency of the dissociation process which, in turn, depends on the condition of the metal surface. Thin oxide films on metal surfaces significantly reduce the ability of hydrogen to dissociate thus the presence of an oxide has the same impact on hydrogen absorption as lowering the hydrogen pressure would have. A typical 1020 steel component exposed to hydrogen gas at one atmosphere pressure and room temperature will dissolve far less than one ppm of hydrogen. However, when the same component is corroded by acid cleaning, exposure to hydrogen sulfide, or simply by exposure to moisture, the concentration of nascent hydrogen on the surface may become quite high and the hydrogen solubility during the exposure may exceed several ppm. A schematic of the effects of time and temperature on hydrogen absorption by low carbon steels exposed to similar concentrations of various acids is shown in Figure 2. Although no hydrogen concentrations are shown in Figure 2, exposure of steels to acidic solutions generally charges more hydrogen into the metal than exposure to hydrogen gas unless the gas pressure is very high. The tendency for acid exposures to charge hydrogen into a metal is one reason the acid based cleaning solutions should be used with caution (or not at all) if hydrogen is known to affect the performance of the alloy. Numerous steel components have absorbed hydrogen, cracked and failed because of acid cleaning operations. The absorbed hydrogen in a metal can be present in either of two locations in the microstructure: interstitial sites in the lattice or extraordinary sites typically associated with crystalline defects. Hydrogen absorption causes the iron lattice to expand because the effective size of the nascent hydrogen atom is larger than the size of the interstitial site. This size difference causes hydrogen to prefer extraordinary sites where the interstitial site size is expanded and the nascent hydrogen is more readily accommodated. Examples of extraordinary sites include grain boundaries, vacancies, dislocations and any other volume where the interstitial sites are dilated. The impact of extraordinary sites on hydrogen absorption is illustrated by Figure 3. Note that for any given time of exposure to 1N sulfuric acid, the amount of hydrogen absorbed increased with increasing cold work. The cold work process increased the dislocation density and vacancy concentrations in the steel and because of the increased concentration of these and other extraordinary sites, the amount of hydrogen absorbed also increased. The concentration of hydrogen at the extraordinary sites in body-centered cubic (ferritic) or body-centered tetragonal (martensitic) steels can greatly exceed the concentration of hydrogen at the normal interstitial sites. Frequently, the hydrogen at extraordinary sites is termed trapped hydrogen and the hydrogen at the normal interstitial sites is termed dissolved or diffusable hydrogen.
The trapped hydrogen concentration is generally in local equilibrium with the dissolved hydrogen concentration. Local equilibrium can be maintained because hydrogen is mobile in most metals, even at room temperature. Because of this mobility hydrogen atoms are able to jump between normal interstitial sites and extraordinary sites. However, because the extraordinary sites are dilated, the residence time for hydrogen in those sites is much higher than its residence time in normal interstitial sites. This difference in residence time often causes the concentration of trapped hydrogen to exceed the concentration of dissolved hydrogen. The site dependent difference in concentration may be many orders of magnitude for bcc and bct steels at room temperature and only a factor of 2 or so for fcc steels. The mobility of hydrogen increases as temperature increases and differences in residence time at the various sites eventually becomes negligible at high temperatures. Additionally, at temperatures much below room temperature the mobility of hydrogen decreases to the point that relocation cannot occur and local equilibrium cannot be maintained. This, very simplified description of hydrogen uptake and migration, can be useful in explaining some of the forms of hydrogen damage to metals. Furthermore, this description can be helpful in recognizing practical solutions to hydrogen induced failures in metallic components. Forms of Hydrogen Damage
Hydrogen Induced Blistering Hydrogen induced blistering occurs during or after hydrogen has been absorbed by the metal. The mobile, nascent hydrogen atoms collect at the extraordinary sites in the metal. Extraordinary sites include the interface between inclusions and the metallic matrix as well as laminations in a wrought structure. Such interfaces are mechanical bonds and provide surfaces inside the metal. As hydrogen collects are this surface the nascent atoms recombine to form a real pressure at the lamination or the inclusion-matrix interface. The magnitude of this pressure will depend on the concentration of absorbed hydrogen in the metal, the trapped-to-dissolved hydrogen ratio and the temperature. If hydrogen was absorbed as the result of exposure to gaseous hydrogen, the interface pressure can never exceed the gaseous hydrogen pressure unless the temperature is higher than the exposure temperature. However, if hydrogen was absorbed because of acid pickling, exposure to hydrogen sulfide, electroplating or cathodic protection the interface pressure may become significant. The difference between gaseous charging and chemical charging of hydrogen is due to differences in the concentration of nascent hydrogen atoms at the